1.
Palani.P.K, Saju.M / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 3, Issue 2, March -April 2013, pp.230-236 Modelling And Optimization Of Process Parameters For Tig Welding Of Aluminium-65032 Using Response Surface Methodology Palani.P.K1 , Saju.M2, Associate Professor 1 , PG Scholar 2 Department of Mechanical Engineering, Government College of Technology, Coimbatore.Abstract Tungsten inert gas welding is one of the properties, exhibits good weld ability and is one ofwidely used techniques for joining ferrous and the most common alloys of aluminium. Chemicalnon ferrous metals. TIG welding offers several composition [1] of Al-65032 is given in table 1advantages like joining of dissimilar metals, low Table 1: Chemical composition of Aluminium –heat affected zone, absence of slag etc. The aim of 65032this paper is to investigate the effect of TIG Al Si Fe Cu Mn Cr Zi Tiwelding process parameters on welding of 97.53 0.4- <0.7 0.15 – <0.15 0.04- <0.25 <0.15Aluminium-65032. Response Surface 0.8 0.4 0.35Methodology was used to conduct the Application of Al – 65032 alloy includesexperiments. The parameters selected for construction of aircraft structures, construction ofcontrolling the process are welding speed, boats, bicycle frames and components, automobilecurrent and gas flow rate. Strength of welded parts, cans for packing of food stuffs and beveragesjoints were tested by a UTM. Percent elongation etc.was also calculated to evaluate the ductility of thewelded joint. From the results of the 2. LITERATURE REVIEWexperiments, mathematical models have been G.Haragopal et al. (2011) [1] used Taguchideveloped to study the effect of process method to study the effect of gasparameters on tensile strength and percent pressure,current,grooveangle and preheat on MIGelongation. Optimization was done to find welding of Aluminium alloy(Al-65032). Theyoptimum welding conditions to maximize tensile indicated that welding current has more effectstrength and percent elongation of welded ultimate tensile strength whereas gas pressure is thespecimen. Confirmation tests were also most significant parameter for proof stress,conducted to validate the optimum parameter elongation and impact energy.settings. G.Padmanaban et al (2011) [2] studied the effect of optimization of pulsed current gas tungstenKeywords: TIG welding, Al-65032, Ultimate arc welding process parameters on tensile strengthTensile Strength, Response Surface Methodology. in AZ31B magnesium alloy. Result showed that maximum tensile strength of 188Mpa was obtained1. INTRODUCTION under the welding condition of peak current of 2101.1 WELDING A, base current of 80A, pulse frequency of 6 Hz and Welding is a fabrication process that joins pulse on time of 50%.materials, usually metals or thermoplastics by R.Satish et al. (2012) [3] studiedcausing coalescence. Gas tungsten arc welding, weldability and process parameter optimization ofGTAW, also known as tungsten inert gas welding, is dissimilar pipe joints using GTAW. Taguchi methodan arc welding process that uses a non consumable was used to formulate the experimental layout toelectrode to produce the weld. Weld area is rank the welding input parameters which affectsprotected from atmospheric contamination by a quality of weld. Results showed that lower heatshielding gas (usually inert gas such as argon) and a input resulted in lower tensile strength and too highfiller material is normally used.GTAW is most heat input also resulted in reduced tensile strength.commonly used to weld thin sections of stainless Dr.Kumar et al (2009) [4] investigated the effect ofsteel and non ferrous metals such as aluminium, process parameters on GTAW for Al-7039 alloy.magnesium and copper alloys. Taguchi method is used to formulate theAluminium based alloys have been widely used in experimental layout to analyze the effect of eachautomobile structures due to their unique properties process parameters on bead geometry.such as high strength to weight ratio. Narongchai Sathavornvichit et al, (2006)1.2 Aluminium – 65032 [5] determined the optimal factors of Flux cored arcAluminium – 65032 is a precipitation hardening welding process for steel ST37.Experiments werealuminium alloy [1], which has good mechanical conducted by central composite design,They found 230 | P a g e
2.
Palani.P.K, Saju.M / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 3, Issue 2, March -April 2013, pp.230-236that optimum conditions were 300ampere of Table 2: Factors & Levelscurrent,30volt of voltage,45mm of stickout and 60 Levelsdegrees of angle. Notation Ugur esme et al.(2009) [6] investigated the Factors -1 0 +1multi response optimization of tungsten inert gaswelding for an optimal parametric combination to Welding speed (mm / S 150 175 200yield favorable bead geometry of welded joints min)using grey relational analysis and Taguchi method.The significance of factors on overall quality Welder current (Amps) I 100 110 120characteristics of the weldment has also been Gas flow rate (LPM) L 10 11 12evaluated quantitatively by the analysis of variance RSM also quantifies relationships among one ormethod. more measured responses and the vital input factors. M.Balasubramanian et al (2009) [7] studied The version 14 of the MINITAB software was usedthe weld pool geometry of pulsed current gas to develop the experimental plan for RSM.tungsten arc welded titanium alloy using centralcomposite design. Mathematical models were 3.2 Central Composite Design (CCD)developed. Lexicographic method was used to The first requirement for RSM involves theoptimize process parameters. design of experiments to achieve adequate and Erdal Karadeniz et al (2007) [8] studied reliable measurement of the response of interest. Tothe effects of various welding parameters on meet this requirement, an appropriate experimentalwelding penetration in ERD emir 6842 steel having design technique has to be employed. The2.5mm thickness welded by robotic gas metal arc experimental design techniques commonly used forwelding. welding current ,welding speed and arc process analysis and modelling are the full factorial,voltage were chosen as process parameters. The partial factorial and central composite designs. Adepth of penetration were measured for each full factorial design requires at least three levels perspecimen and effect of these parameters on variable to estimate the coefficients of the quadraticpenetration were researched. From the study, it is terms in the response model A partial factorialfound that increasing welding current increased the design requires fewer experiments than the fulldepth of penetration. factorial design However, the former is particularly D.S.Nagesh et al (2002) [9] studied that useful if certain variables are already known tobead geometry and penetration are important show no interaction. An effective alternative tophysical characteristic of a weldament. It was factorial design is central composite design (CCD),observed that high arc travel rate or low arc power [5, 13-14] requires many fewer tests than the fullnormally produce poor fusion. A neural network factorial design and has been shown to be sufficientwas developed for estimating weld bead and to describe the majority of steady-state processpenetration geometric parameters. responses. Hence in this study, it was decided to use From the literatures, it is observed that only CCD to design the experiments. Hence the totalfew works have been reported on the study of TIG number of tests required for the three independentwelding process parameters for welding of variables is 23 + (2x3 + 6 = 20. Once the desiredAluminium-65032. Therefore the aim of the present ranges of values of the variables are defined, theystudy is to investigate the effect of TIG welding are coded to lie at ±1 for the factorial points, 0 forprocess parameters on the welding of Al-65032.The the center points and ±p for the axial points.experiments were conducted using a statisticaltechnique called Design of Experiments (DOE). 3.4 Factors and Levels In this study three parameters have been chosen for analysis. They are welding speed,3. METHODOLOGY OF welding current and gas flow rate [3-4, 12]. SeveralINVESTIGATION trial runs were conducted to determine the range of3.1 Response Surface Methodology (RSM) parameters. The levels for parameters finally Response Surface Methodology (RSM) is a chosen are shown in table 2.collection of statistical and mathematical techniquesuseful for developing, improving, and optimizingprocesses [2, 10-11]. With this technique, the effectof two or more factors on quality criteria can beinvestigated and optimum values are obtained. InRSM design there should be at least three levels foreach factor. 231 | P a g e
3.
Palani.P.K, Saju.M / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 3, Issue 2, March -April 2013, pp.230-236Table 3: central Composite Design Matrix Welding process has been carried out in TIG Gas flow welding machine. Experiments were conductedExp Welding speed Welding based on central composite design matrix [5] rateNo. (mm / min) current ( A) which is given in Table 4. ( LPM)1. -1 -1 -12. 1 -1 -13. -1 1 -14. 1 1 -15. -1 -1 16. 1 -1 17. -1 1 18. 1 1 19. -1 0 010. 1 0 011. 0 -1 012. 0 1 013. 0 0 -114. 0 0 1 Fig. 1 Photos of Welded Specimen15. 0 0 016. 0 0 0 4.2 Tensile Testing17. 0 0 0 The ultimate tensile strength of the18. 0 0 0 machined specimen were tested in the calibrated19. 0 0 0 universal tensile testing machine. Percent elongation20. 0 0 0 was also calculated. Tensile test carried out according to ASTM standards, using specimenTable 4: Experimental Design Variables prepared as shown in Fig.2 Welding Welding Gas flowExp speed current rateNo. ( mm / min) (A) (LPM)1. 150 100 102. 200 100 103. 150 120 104. 200 120 105. 150 100 126. 200 100 12 Fig.2 Dimensions of tensile test specimen 4.2.1 Test Specimen7. 150 120 12 Welded joints were machined for conducting tensile8. 200 120 12 test. Test specimen prepared according to ASTM9. 150 110 11 Standards is shown in Fig 3.10. 200 110 1111. 175 100 1112. 175 120 1113. 175 110 1014. 175 110 1215. 175 110 1116. 175 110 1117. 175 110 1118. 175 110 1119. 175 110 1120. 175 110 114. EXPERIMENTAL WORK Fig.3 Test Specimen4.1 Experimental Procedure The Tensile test was carried out in the Welding specimen has been prepared to servo controlled universal testing machine withfabricate TIG welded joints. Aluminium alloy 65032 1000 KN load capacity. The specimen is loaded atspecimen (75mm x 75mm x 3mm) in the specified the rate of 0.1KN/Min. Due to the pulling effect ofdimension was considered for welding of square machine, tensile specimen undergoes deformation.butt joints. Twenty specimens were tested at each condition, 232 | P a g e
4.
Palani.P.K, Saju.M / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 3, Issue 2, March -April 2013, pp.230-236 ultimate tensile strength and percent elongation were calculated Contribution Source DF SS MS F P (%) Regression 9 1465.6 1465.6 6.55 0.004 85.49 Model Linear 3 999.83 999.83 13.40 0.001 58 Square 3 452.52 452.52 6.07 0.013 26.39 Interaction 3 13.25 13.25 0.18 0.909 0.77 Residual 10 248.64 248.64 - - - Error Lack of Fit 5 222.24 222.24 8.42 0.018 12.96 Pure Error 5 26.4 26.4 - Total 19 1714.24 - 100 5.3 Model coefficients for UTS. Fig.4 Specimen after tensile test Table 7 Table 5:. Tensile strength and % Elongation values Term Coef Term Coef Term Coef Gas Constant Welding Welding Welding Welding TensileExp. Flow % 96.138 speed*welding 10.6045 speed*welding 0.1250 Speed Current StrengthNo Rate Elongation speed current (Mm/Min) (Amps) (Mpa) (Lpm) Welding Welding Welding1 150 100 10 112.7 6.12 - speed -9.75 current*welding -2.4955 speed*gas2 200 100 10 98.6 5.8 1.2750 current flow rate3 150 120 10 109.3 6.1 Welding Welding4 200 120 10 88 5.55 Gas flow rate current -2.17 0.3545 current*gas 0.12505 150 100 12 122.6 6.25 *gas flow rate flow rate6 200 100 12 95.7 5.6 Gas7 150 120 12 112 6.15 flow 0.46 - - - -8 200 120 12 93.3 5.7 rate9 150 110 11 117.3 6.20 Table 6 shows ANOVA table corresponding to10 200 110 11 100.8 5.9 ultimate tensile strength. Linear has great11 175 100 11 93.3 5.65 percentage of contribution on UTS and Interaction12 175 120 11 98.6 5.85 has less percentage of contribution on UTS. Table 7 shows estimated model coefficients for13 175 110 10 104 5.95 ultimate tensile strength.14 175 110 12 93.6 5.65 5.4 Estimated regression Model for UTS15 175 110 11 96 5.75 From Regression analysis, a mathematical model for16 175 110 11 96 5.75 predicting UTS in terms of welding speed, current17 175 110 11 93 5.6 and gas flow rate is developed and is given below.18 175 110 11 96 5.7 UTS = 96.138 – 9.75 x S – 2.17 x I + 0.46x L +19 175 110 11 90.6 5.55 10.6045 x S2 – 2.4955 x I2 + 0.3545 x L2 + 0.1250 x20 175 110 11 96 5.75 S xI – 1.2750 x S x L + 0.1250 x A x L. 5. RESULTS AND DISCUSSION 5.5 Analysis of variance for % Elongation 5.1 Analysis of variance Table 8: ANOVA For %Elongation Analysis of variance (ANOVA) is similar S = 0.1397, R-sq = 80.0% R-sq (adj) = 75.21% to regression in that it is used to investigate and model the relationship between a response variable and one or more independent variables. In this study general linear model is used to determine the influence of welding speed, current and gas flow rate on ultimate tensile strength and % Elongation. 5.2 Analysis of variance for UTS Table 6: ANOVA For UTS S = 4.986, R-sq = 85.5% R-sq (adj) = 75.1% 233 | P a g e
5.
Palani.P.K, Saju.M / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 3, Issue 2, March -April 2013, pp.230-236 Table 10: Response optimization for process Contribution parameterSource DF SS MS F P (%)Regression 9 0.77857 0.86508 4.43 0.015 80.4 OptimumModel Predicte Combination Para Go d Weldi Gas Curren Target Lower UpperLinear 3 0.51867 0.1728 8.86 0.004 52.37 meters al Respons ng flow e speed rate tSquare 3 0.24406 0.081 4.17 0.037 24.74 Tensile Ma 108.38 11.9 122. 122. 150 88 119.1298 strength x 5 9 6 6Interaction 3 0.01584 0.0052 0.27 0.845 0.0162 % Ma 108.38 11.9 5.5Residual 10 0.19509 0.019 - - - Elongat 150 6.25 6.25 6.21 x 5 9 5Error ionLack of Fit 5 0.15675 0.031 4.09 0.047 -Pure Error 5 0.03833 0.007 - - -Total 19 0.97366 - - 100 5.6 Model Coefficients For Percent Elongation. Table 9Term Coef Term Coef Term Coef Fig 5. Optimization using MINITAB VI4 SoftwareConstan Welding Welding -t 5.730 speed*welding 0.2486 speed*weldin 0.00375 5.9 Effect of process parameters on UTS speed g current The main effects of the plot, for UTS withWelding Welding Welding the process parameter of welding speed, current and -speed -0.227 current*weldin speed*gas -0.2875 gas flow rate were shown in Fig.5.2. Graph shows 0.05136 g current flow rate that UTS decreases from 115 MPa to 95 MPa. whenWelding Welding welding speed increases from 150mm/min to 200 Gas flow rate -current -0.017 current*gas 0.03375 mm/min,because of less penetration depth. UTS *gas flow rate 0.00136 flow rate decreases from 105 MPa to 101MPa when currentGas changes from 100 Amps to 120 Amps, due to the 0.007flow result of increased input heat associated with the use of higher current. As gas flow rate changes from 10 Table 8 shows the ANOVA table LPM to 12 LPM,UTS increases from 103Mpa to corresponding to % Elongation. This table shows 104Mpa,due to decrease in the porosity level of that main effects of welding speed, current and gas weld metal. Fig 7 is contour plot, is a graphic flow rate are all significant with respect to percent representation of the relationship among three elongation. Table 9 shows estimated model numeric variables in two dimensions coefficients for percent elongation. 5.7 Estimated Regression model for % Elongation %Elongation = 5.730 – 0.227 x S - 0.017 x I – 0.007 x L + 0.2486 x S2 - 0.05136 x I2 - 0.00136 x L 2 - 0.00375 x S x I – 0.2875 x S xL + 0.03375 x I x L. 5.8 Optimization of process Parameters One of the most important aims of experiments related to welding is to achieve high value of tensile strength and Elongation. The response surface optimization is a technique for determining best welding parameter combination[6- 7,13]. Here the goal is to maximize UTS and % Elongation. RSM optimization result for UTS and % Elongation is shown in Fig 5. Optimum parameters obtained are shown in table 1 Fig.6 Main effect plot for UTS 234 | P a g e
6.
Palani.P.K, Saju.M / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 3, Issue 2, March -April 2013, pp.230-236 6. CONCLUSION The effect of TIG welding parameters like welding speed, current and gas flow rate on ultimate tensile strength and percent elongation in welding of Al-65032 has been studied. Experiments were conducted using central composite design matrix and mathematical models have been developed. From the study it was observed that welding speed has the most significant effect on both UTS and percent Elongation followed by welding current. However gas flow rate has least significant influence on both UTS and percent elongation. Optimization was done to maximize UTS and percent elongation. Predicted properties at optimum condition are verified with a confirmation test andFig.7 Contour plot for UTS are found within the limits.5.10 Effect of Process parameters on Percent REFERENCESElongation [1] G.Hargopal, P.V.R.Ravindra reddy, The main effect plot shows that value of “Parameter design for MIG welding of Al-percent elongation decreases as welding speed 65032 alloy using Taguchi technique”,increases from 150mm/min to 200mm/min. it is due Journal of scientific and industrialto the fact that orientation of the grains has the research, vol 70,2011,pp.844-850.predominant effect on the decreased ductility with [2] G.Padmanaban, V.Balasubramanian,increasing travel speed. As current changes from “Optimization of pulsed current gas100A to 120 Amps, percent elongation decreases tungsten arc welding process parameters todue to high heat input. When gas flow rate increases attain maximum tensile strength in AZ31Bfrom 10 LPM to 12 LPM,percent elongation magnesium alloy”, Trans.Non ferrousdecreases. Fig. 9 shows the contour plot for percent Met.soc.china 21,2011,467-476.Elongation at Constant welding speed, current and [3] R.Satish, B.Naveen, “Weldability andgas flow rate. process parameter optimization of dissimilar pipe joints using GTAW”.International Journal of Engineering research and applications, vol2,2012, pp.I2525-2530. [4] Dr.P.Kunar, Dr.K.P.Kohle, “Process optimization of pulsed GTAW process for Al-7039 alloy using Ar+He Gas “,IE(I) Journal-MC vol 9,2011. [5] Narongchai Sathavornvichit,et al “Central composite design in Optimization of the factors of automatic flux cored arc welding for steel ST37”Regional conference onFig. 8 Main effects plot for percent elongation mathematics, university sains,Malaysia,june 13-15,2006. [6] Ugur Esme, Melih Bayramoglu, “Optimization of weld bead geometry in TIG welding process using grey relation analysis and taguchi method”, Original scientific article MTAEC9, 43(3),2009,pp 143-149. [7] M.Balasubramanian,V.Jayabalan,“Predictio n and optimization of Pulsed current gas tungsten arc welding process parameters to obtain sound weld pool geometry in Titanium alloy using lexicographic method”,JMEPEG 18,2009,pp 871-877. [8] Erdal Karadeniz, Ugur Ozsarac, “The effect of process parameters on penetrationFig 9. Contour plot for % Elongation 235 | P a g e
7.
Palani.P.K, Saju.M / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 3, Issue 2, March -April 2013, pp.230-236 in gas metal arc welding process”, Materials and designs 28,pp 649-656,2007.[9] D.S.Nagesh, G.L.Datta, “Prediction of weld bead geometry and penetration in shielded metal arc welding using artificial neural network”, Journal of material processing technology, 123,pp 303- 312,2002[10] P.K.Palani, N.Murugan, “optimization of weld bead geometry for stainless steel claddings deposited by FCAW” Journal of material processing technology,vol 190,2007,pp.291-299[11] P.K Palani, N.Murugan, “Modeling and analysis of pitting corrosion resistance of stainless steel overlays deposited by Flux cored arc welding”. Journal of surface engineering, vol 24, 2008, pp 422-430.[12] B.Chan, J.Pacey, “Modelling gas metal arc weld geometry using artificial neural network technology”, Canadian metallurgical quarterly, vol 38, 1999.[13] Parmer R.S., Welding Engineering and Technology, Khanna publishers,1997.[14] P K Palani, N Murugan, “Prediction of Delta ferrite content and effect of welding process Parameters in claddings by FCAW.Materials and Manufacturing processes”, 21:431-438,2005.[15] P.K.Palani, N.Murugan, “Development of mathematical models for prediction of Weld bead geometry in cladding by flux Cored arc welding”. Int J Adv Manuf Technol ,2006, 30: 669-676 236 | P a g e
Be the first to comment